# Electronic Supplementary Material (ESI) for CrystEngComm.
# This journal is © The Royal Society of Chemistry 2021

####################################################################### 
# 
# This file contains crystal structure data downloaded from the 
# Cambridge Structural Database (CSD) hosted by the Cambridge 
# Crystallographic Data Centre (CCDC).
# 
# Full information about CCDC data access policies and citation 
# guidelines are available at http://www.ccdc.cam.ac.uk/access/V1 
# 
# Audit and citation data items may have been added by the CCDC. 
# Please retain this information to preserve the provenance of 
# this file and to allow appropriate attribution of the data. 
# 
#######################################################################

data_wk627
_database_code_depnum_ccdc_archive 'CCDC 2102365'
loop_
_audit_author_name
_audit_author_address
'Pavel Abramov'
;Nikolaev Institute of Inorganic Chemistry SB RAS
Russia
;
_audit_update_record             
;
2021-08-09 deposited with the CCDC.	2021-11-12 downloaded from the CCDC.
;

_audit_creation_method           SHELXL-2017/1
_shelx_SHELXL_version_number     2017/1
_chemical_name_systematic        ?
_chemical_name_common            ?
_chemical_melting_point          ?
_chemical_formula_moiety         ?
_chemical_formula_sum            'C21.80 H130.80 Cl3 Mo132 N65.40 O581.40 Se30'
_chemical_formula_weight         25751.54

loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
C C 0.0047 0.0021 'ShelXle (H\"ubschle, 2011)'
H H 0.0000 0.0000 'ShelXle (H\"ubschle, 2011)'
N N 0.0086 0.0042 'ShelXle (H\"ubschle, 2011)'
O O 0.0148 0.0078 'ShelXle (H\"ubschle, 2011)'
Se Se -0.4874 2.7657 'ShelXle (H\"ubschle, 2011)'
Mo Mo -1.2345 0.8540 'ShelXle (H\"ubschle, 2011)'
Cl Cl 0.1484 0.1585 'ShelXle (H\"ubschle, 2011)'

_space_group_crystal_system      trigonal
_space_group_IT_number           167
_space_group_name_H-M_alt        'R -3 c :H'
_space_group_name_Hall           '-R 3 2"c'

_shelx_space_group_comment       
;
The symmetry employed for this shelxl refinement is uniquely defined
by the following loop, which should always be used as a source of
symmetry information in preference to the above space-group names.
They are only intended as comments.
;

loop_
_space_group_symop_operation_xyz
'x, y, z'
'-y, x-y, z'
'-x+y, -x, z'
'y, x, -z+1/2'
'x-y, -y, -z+1/2'
'-x, -x+y, -z+1/2'
'x+2/3, y+1/3, z+1/3'
'-y+2/3, x-y+1/3, z+1/3'
'-x+y+2/3, -x+1/3, z+1/3'
'y+2/3, x+1/3, -z+5/6'
'x-y+2/3, -y+1/3, -z+5/6'
'-x+2/3, -x+y+1/3, -z+5/6'
'x+1/3, y+2/3, z+2/3'
'-y+1/3, x-y+2/3, z+2/3'
'-x+y+1/3, -x+2/3, z+2/3'
'y+1/3, x+2/3, -z+7/6'
'x-y+1/3, -y+2/3, -z+7/6'
'-x+1/3, -x+y+2/3, -z+7/6'
'-x, -y, -z'
'y, -x+y, -z'
'x-y, x, -z'
'-y, -x, z-1/2'
'-x+y, y, z-1/2'
'x, x-y, z-1/2'
'-x+2/3, -y+1/3, -z+1/3'
'y+2/3, -x+y+1/3, -z+1/3'
'x-y+2/3, x+1/3, -z+1/3'
'-y+2/3, -x+1/3, z-1/6'
'-x+y+2/3, y+1/3, z-1/6'
'x+2/3, x-y+1/3, z-1/6'
'-x+1/3, -y+2/3, -z+2/3'
'y+1/3, -x+y+2/3, -z+2/3'
'x-y+1/3, x+2/3, -z+2/3'
'-y+1/3, -x+2/3, z+1/6'
'-x+y+1/3, y+2/3, z+1/6'
'x+1/3, x-y+2/3, z+1/6'

_cell_length_a                   50.337(7)
_cell_length_b                   50.337(7)
_cell_length_c                   61.099(12)
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_volume                     134072(46)
_cell_formula_units_Z            6
_cell_measurement_temperature    100(2)
_cell_measurement_reflns_used    969
_cell_measurement_theta_min      2.23
_cell_measurement_theta_max      28.10

_exptl_crystal_description       block
_exptl_crystal_colour            black
_exptl_crystal_density_meas      ?
_exptl_crystal_density_method    ?
_exptl_crystal_density_diffrn    1.914
_exptl_crystal_F_000             71914
_exptl_transmission_factor_min   ?
_exptl_transmission_factor_max   ?
_exptl_crystal_size_max          0.300
_exptl_crystal_size_mid          0.200
_exptl_crystal_size_min          0.200
_exptl_absorpt_coefficient_mu    4.160
_shelx_estimated_absorpt_T_min   0.368
_shelx_estimated_absorpt_T_max   0.490
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_correction_T_min  0.8462
_exptl_absorpt_correction_T_max  1.0000
_exptl_absorpt_process_details   'XDS (Kabsch, 2010)'
_exptl_absorpt_special_details   ?
_diffrn_ambient_temperature      100(2)
_diffrn_radiation_wavelength     0.79272
_diffrn_radiation_type           synchrotron
_diffrn_source                   synchrotron
_diffrn_measurement_device_type  'Rayonix SX-165 CCD'
_diffrn_measurement_method       'φ scan'
_diffrn_detector_area_resol_mean 12.4
_diffrn_reflns_number            287412
_diffrn_reflns_av_unetI/netI     0.0372
_diffrn_reflns_av_R_equivalents  0.0775
_diffrn_reflns_limit_h_min       -65
_diffrn_reflns_limit_h_max       59
_diffrn_reflns_limit_k_min       -65
_diffrn_reflns_limit_k_max       65
_diffrn_reflns_limit_l_min       -78
_diffrn_reflns_limit_l_max       79
_diffrn_reflns_theta_min         1.428
_diffrn_reflns_theta_max         31.004
_diffrn_reflns_theta_full        28.401
_diffrn_measured_fraction_theta_max 0.996
_diffrn_measured_fraction_theta_full 0.999
_diffrn_reflns_Laue_measured_fraction_max 0.996
_diffrn_reflns_Laue_measured_fraction_full 0.999
_diffrn_reflns_point_group_measured_fraction_max 0.996
_diffrn_reflns_point_group_measured_fraction_full 0.999
_reflns_number_total             34107
_reflns_number_gt                23366
_reflns_threshold_expression     'I > 2σ(I)'
_reflns_Friedel_coverage         0.000
_reflns_Friedel_fraction_max     .
_reflns_Friedel_fraction_full    .

_reflns_special_details          
;
 Reflections were merged by SHELXL according to the crystal
 class for the calculation of statistics and refinement.
 
 _reflns_Friedel_fraction is defined as the number of unique
 Friedel pairs measured divided by the number that would be
 possible theoretically, ignoring centric projections and
 systematic absences.
;
_computing_data_collection       'Marccd (Doyle, 2011)'
_computing_cell_refinement       'XDS (Kabsch, 2010)'
_computing_data_reduction        'XDS (Kabsch, 2010)'
_computing_structure_solution    'SHELXT-2018 (Sheldrick, 2015)'
_computing_structure_refinement  'SHELXL-2018 (Sheldrick, 2015)'
_computing_molecular_graphics    'ShelXle (Hübschle, 2011)'
_computing_publication_material  'CIFTAB (Sheldrick, 2015)'
_refine_special_details          ?
_refine_ls_structure_factor_coef Fsqd
_refine_ls_matrix_type           full
_refine_ls_weighting_scheme      calc
_refine_ls_weighting_details     
'w=1/[σ²(Fo²)+(0.2000P)²] where P=(Fo²+2Fc²)/3'
_atom_sites_solution_primary     dual
_atom_sites_solution_secondary   difmap
_atom_sites_solution_hydrogens   geom
_refine_ls_hydrogen_treatment    constr
_refine_ls_extinction_method     none
_refine_ls_extinction_coef       .
_refine_ls_number_reflns         34107
_refine_ls_number_parameters     1294
_refine_ls_number_restraints     90
_refine_ls_R_factor_all          0.1236
_refine_ls_R_factor_gt           0.0921
_refine_ls_wR_factor_ref         0.3187
_refine_ls_wR_factor_gt          0.2929
_refine_ls_goodness_of_fit_ref   1.211
_refine_ls_restrained_S_all      1.211
_refine_ls_shift/su_max          0.002
_refine_ls_shift/su_mean         0.000

loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_site_symmetry_order
_atom_site_calc_flag
_atom_site_refinement_flags_posn
_atom_site_refinement_flags_adp
_atom_site_refinement_flags_occupancy
_atom_site_disorder_assembly
_atom_site_disorder_group
C1 C 0.4097(5) 0.2310(6) 0.2688(4) 0.105(6) Uani 1 1 d . U . . .
C2 C 0.6648(4) 0.4914(4) 0.1872(3) 0.090(5) Uani 1 1 d . . . . .
C3 C 0.7638(3) 0.5936(4) 0.3997(2) 0.073(4) Uani 1 1 d . . . . .
C4 C 0.666667 0.333333 0.1371(5) 0.0782(13) Uani 1 3 d S TU P . .
N1 N 0.4067(5) 0.2468(5) 0.2852(4) 0.118(6) Uani 1 1 d . U . . .
H1A H 0.400652 0.238212 0.298167 0.142 Uiso 1 1 calc R U . . .
H1B H 0.410871 0.265798 0.283125 0.142 Uiso 1 1 calc R U . . .
N2 N 0.4042(4) 0.2035(5) 0.2702(3) 0.114(6) Uani 1 1 d . U . . .
H2A H 0.398052 0.193623 0.282746 0.137 Uiso 1 1 calc R U . . .
H2B H 0.406599 0.194379 0.258730 0.137 Uiso 1 1 calc R U . . .
N3 N 0.4200(4) 0.2464(4) 0.2479(3) 0.107(5) Uani 1 1 d . U . . .
H3A H 0.422322 0.236750 0.236696 0.128 Uiso 1 1 calc R U . . .
H3B H 0.423941 0.265438 0.246364 0.128 Uiso 1 1 calc R U . . .
N4 N 0.6907(4) 0.4951(4) 0.1813(3) 0.093(4) Uani 1 1 d . U . . .
H4A H 0.707660 0.510005 0.187054 0.111 Uiso 1 1 calc R U . . .
H4B H 0.691617 0.482707 0.171591 0.111 Uiso 1 1 calc R U . . .
N5 N 0.6390(3) 0.4692(4) 0.1801(3) 0.104(6) Uani 1 1 d . . . . .
H5A H 0.621561 0.466940 0.185057 0.125 Uiso 1 1 calc R U . . .
H5B H 0.638811 0.456265 0.170291 0.125 Uiso 1 1 calc R U . . .
N6 N 0.6653(5) 0.5099(4) 0.2011(3) 0.112(5) Uani 1 1 d . U . . .
H6A H 0.682896 0.524421 0.206316 0.134 Uiso 1 1 calc R U . . .
H6B H 0.647978 0.508331 0.205701 0.134 Uiso 1 1 calc R U . . .
N7 N 0.7902(3) 0.5972(3) 0.3961(2) 0.077(4) Uani 1 1 d . . . . .
H7A H 0.799506 0.592562 0.406321 0.092 Uiso 1 1 calc R U . . .
H7B H 0.799142 0.604212 0.383359 0.092 Uiso 1 1 calc R U . . .
N8 N 0.7491(3) 0.5830(3) 0.4186(2) 0.079(4) Uani 1 1 d . . . . .
H8A H 0.757674 0.578162 0.429240 0.095 Uiso 1 1 calc R U . . .
H8B H 0.730768 0.580853 0.420471 0.095 Uiso 1 1 calc R U . . .
N9 N 0.7491(3) 0.6003(4) 0.3833(2) 0.086(4) Uani 1 1 d . . . . .
H9A H 0.758089 0.607021 0.370524 0.104 Uiso 1 1 calc R U . . .
H9B H 0.730787 0.597927 0.385648 0.104 Uiso 1 1 calc R U . . .
N10 N 0.6406(3) 0.3332(3) 0.1367(3) 0.093(5) Uani 1 1 d . . . . .
H10A H 0.623173 0.315734 0.136193 0.111 Uiso 1 1 calc R U . . .
H10B H 0.640533 0.350680 0.136992 0.111 Uiso 1 1 calc R U . . .
O1 O 0.69025(19) 0.58364(19) 0.26897(13) 0.0532(18) Uani 1 1 d . . . . .
O2 O 0.55234(19) 0.35825(19) 0.15409(12) 0.0521(18) Uani 1 1 d . . . . .
O3 O 0.7067(2) 0.60088(18) 0.30455(13) 0.0539(18) Uani 1 1 d . . . . .
O4 O 0.6201(2) 0.5567(2) 0.30499(13) 0.0550(19) Uani 1 1 d . . . . .
O5 O 0.7475(2) 0.62318(19) 0.33828(14) 0.0554(19) Uani 1 1 d . . . . .
O6 O 0.52530(18) 0.37434(19) 0.17581(12) 0.0488(17) Uani 1 1 d . . . . .
O7 O 0.5710(2) 0.2999(2) 0.13287(14) 0.0571(19) Uani 1 1 d . . . . .
O8 O 0.6012(2) 0.4149(2) 0.14790(13) 0.0558(19) Uani 1 1 d . . . . .
O9 O 0.5854(2) 0.3932(2) 0.18999(13) 0.058(2) Uani 1 1 d . . . . .
O10 O 0.5172(2) 0.4144(2) 0.20063(13) 0.0556(19) Uani 1 1 d . . . . .
O11 O 0.42959(19) 0.1259(2) 0.22697(14) 0.058(2) Uani 1 1 d . . . . .
O12 O 0.5598(2) 0.5162(2) 0.29615(14) 0.059(2) Uani 1 1 d . . . . .
O13 O 0.53860(19) 0.33199(19) 0.19637(12) 0.0504(17) Uani 1 1 d . . . . .
O14 O 0.5792(2) 0.5355(2) 0.33839(14) 0.058(2) Uani 1 1 d . . . . .
O15 O 0.5859(2) 0.3316(2) 0.17137(14) 0.060(2) Uani 1 1 d . . . . .
O16 O 0.6316(2) 0.5377(2) 0.22711(14) 0.0549(19) Uani 1 1 d . . . . .
O17 O 0.6021(2) 0.4972(2) 0.28772(16) 0.061(2) Uani 1 1 d . . . . .
O18 O 0.4388(2) 0.1652(2) 0.28715(15) 0.059(2) Uani 1 1 d . . . . .
O19 O 0.4110(2) 0.2976(2) 0.25847(14) 0.058(2) Uani 1 1 d . . . . .
O20 O 0.4672(2) 0.2279(2) 0.17518(15) 0.061(2) Uani 1 1 d . . . . .
O21 O 0.4772(2) 0.4334(2) 0.37071(14) 0.058(2) Uani 1 1 d . . . . .
O22 O 0.6642(2) 0.53700(18) 0.30097(13) 0.0537(18) Uani 1 1 d . . . . .
O23 O 0.6319(2) 0.56936(19) 0.36501(14) 0.0569(19) Uani 1 1 d . . . . .
O24 O 0.72866(19) 0.4801(2) 0.14809(13) 0.0547(18) Uani 1 1 d . . . . .
O25 O 0.4410(2) 0.3624(2) 0.25773(15) 0.062(2) Uani 1 1 d . . . . .
O26 O 0.5996(2) 0.4884(2) 0.19836(14) 0.0568(19) Uani 1 1 d . . . . .
O27 O 0.6951(2) 0.6034(2) 0.36527(14) 0.058(2) Uani 1 1 d . . . . .
O28 O 0.5479(2) 0.3318(2) 0.11215(14) 0.062(2) Uani 1 1 d . . . . .
O29 O 0.7018(2) 0.4554(2) 0.10785(14) 0.066(2) Uani 1 1 d . . . . .
O30 O 0.7021(2) 0.56222(19) 0.33942(15) 0.058(2) Uani 1 1 d . . . . .
O31 O 0.74566(19) 0.4750(2) 0.19026(13) 0.0543(18) Uani 1 1 d . . . . .
O32 O 0.4854(2) 0.2925(2) 0.22172(14) 0.0574(19) Uani 1 1 d . . . . .
O33 O 0.4351(2) 0.2466(2) 0.20064(15) 0.060(2) Uani 1 1 d . . . . .
O34 O 0.3966(2) 0.1437(2) 0.25236(14) 0.061(2) Uani 1 1 d . . . . .
O35 O 0.5879(3) 0.5687(3) 0.27221(16) 0.073(3) Uani 1 1 d . . . . .
O36 O 0.4119(2) 0.1930(2) 0.22542(14) 0.058(2) Uani 1 1 d . . . . .
O37 O 0.6290(2) 0.4181(2) 0.10814(13) 0.063(2) Uani 1 1 d . . . . .
O38 O 0.4249(2) 0.2843(3) 0.17403(17) 0.070(2) Uani 1 1 d . . . . .
O39 O 0.6622(2) 0.6143(2) 0.28899(15) 0.062(2) Uani 1 1 d . . . . .
O40 O 0.7093(3) 0.6457(2) 0.33335(16) 0.068(2) Uani 1 1 d . . . . .
O41 O 0.6168(3) 0.5971(2) 0.33432(18) 0.073(3) Uani 1 1 d . . . . .
O42 O 0.5456(2) 0.4057(2) 0.13586(15) 0.066(2) Uani 1 1 d . . . . .
O43 O 0.7843(2) 0.5279(2) 0.13593(15) 0.066(2) Uani 1 1 d . . . . .
O44 O 0.6635(2) 0.5986(2) 0.23496(16) 0.066(2) Uani 1 1 d . . . . .
O45 O 0.4712(2) 0.3770(2) 0.17390(15) 0.065(2) Uani 1 1 d . . . . .
O46 O 0.4649(2) 0.4701(2) 0.34258(16) 0.064(2) Uani 1 1 d . . . . .
O47 O 0.4003(2) 0.3281(3) 0.22262(17) 0.072(3) Uani 1 1 d . . . . .
O48 O 0.5403(2) 0.4702(2) 0.17917(15) 0.065(2) Uani 1 1 d . . . . .
O49 O 0.5237(2) 0.5278(2) 0.32432(16) 0.066(2) Uani 1 1 d . . . . .
O50 O 0.3537(2) 0.0919(2) 0.27231(15) 0.066(2) Uani 1 1 d . . . . .
O51 O 0.5732(3) 0.4298(2) 0.21902(16) 0.074(3) Uani 1 1 d . . . . .
O52 O 0.3820(2) 0.1320(2) 0.20870(17) 0.069(2) Uani 1 1 d . . . . .
O53 O 0.6363(2) 0.3957(3) 0.16975(14) 0.070(3) Uani 1 1 d . . . . .
O54 O 0.6949(2) 0.4258(2) 0.16960(14) 0.070(2) Uani 1 1 d . . . . .
O55 O 0.4037(2) 0.1907(2) 0.17916(17) 0.070(2) Uani 1 1 d . . . . .
O56 O 0.4897(2) 0.3308(2) 0.14408(14) 0.059(2) Uani 1 1 d . . . . .
O57 O 0.4762(2) 0.2325(2) 0.21900(17) 0.074(3) Uani 1 1 d . . . . .
O58 O 0.3789(2) 0.3281(3) 0.27075(16) 0.069(2) Uani 1 1 d . . . . .
O59 O 0.4742(2) 0.3310(3) 0.25072(16) 0.081(3) Uani 1 1 d . . . . .
O60 O 0.52643(19) 0.30494(19) 0.15405(12) 0.0518(17) Uani 1 1 d . . . . .
O61 O 0.48276(19) 0.2878(2) 0.17593(13) 0.0556(19) Uani 1 1 d . . . . .
O62 O 0.48162(19) 0.3309(2) 0.18960(13) 0.0557(19) Uani 1 1 d . . . . .
O63 O 0.6663(2) 0.3978(2) 0.12994(15) 0.059(2) Uani 1 1 d . . . . .
O64 O 0.6364(2) 0.5562(2) 0.26935(14) 0.0545(19) Uani 1 1 d . . . . .
O65 O 0.5682(2) 0.4348(2) 0.17466(14) 0.057(2) Uani 1 1 d . . . . .
O66 O 0.5230(2) 0.3696(2) 0.22167(15) 0.058(2) Uani 1 1 d . . . . .
O67 O 0.6633(2) 0.58324(19) 0.32700(14) 0.0543(19) Uani 1 1 d . . . . .
O68 O 0.6036(2) 0.3652(2) 0.13308(13) 0.0552(19) Uani 1 1 d . . . . .
O69 O 0.4649(2) 0.3619(2) 0.21678(13) 0.0549(19) Uani 1 1 d . . . . .
O70 O 0.6252(2) 0.5219(2) 0.33892(16) 0.064(2) Uani 1 1 d . . . . .
O71 O 0.4453(2) 0.1738(2) 0.19863(15) 0.059(2) Uani 1 1 d . . . . .
O72 O 0.5472(2) 0.4679(2) 0.22548(15) 0.063(2) Uani 1 1 d . . . . .
O73 O 0.6653(2) 0.4505(2) 0.14480(14) 0.058(2) Uani 1 1 d . . . . .
O74 O 0.6647(2) 0.5228(2) 0.25579(15) 0.063(2) Uani 1 1 d . . . . .
O75 O 0.5067(2) 0.4674(2) 0.31207(15) 0.065(2) Uani 1 1 d . . . . .
O76 O 0.5264(2) 0.4869(2) 0.35502(14) 0.060(2) Uani 1 1 d . . . . .
O77 O 0.4348(2) 0.2992(2) 0.21764(15) 0.060(2) Uani 1 1 d . . . . .
O78 O 0.5801(2) 0.5162(2) 0.25327(14) 0.057(2) Uani 1 1 d . . . . .
O79 O 0.5769(2) 0.5291(2) 0.20923(15) 0.062(2) Uani 1 1 d . . . . .
O80 O 0.5644(2) 0.4772(2) 0.32546(19) 0.073(3) Uani 1 1 d . . . . .
O81 O 0.6030(3) 0.4786(2) 0.24362(17) 0.070(3) Uani 1 1 d . . . . .
O82 O 0.4585(2) 0.1839(2) 0.24389(16) 0.066(2) Uani 1 1 d . . . . .
O83 O 0.5159(2) 0.4292(2) 0.3405(2) 0.078(3) Uani 1 1 d . . . . .
O84 O 0.4570(2) 0.3324(3) 0.29042(16) 0.076(3) Uani 1 1 d . . . . .
O86 O 0.5979(5) 0.6210(5) 0.2981(4) 0.055(5) Uiso 0.4 1 d . . P . .
O87 O 0.4869(5) 0.4649(5) 0.2098(4) 0.062(5) Uiso 0.4 1 d . . P . .
O88 O 0.4790(6) 0.4924(6) 0.2778(5) 0.072(6) Uiso 0.4 1 d . . P . .
O89 O 0.5168(4) 0.2216(5) 0.2368(4) 0.171(9) Uani 1 1 d . . . . .
O90 O 0.4861(5) 0.2382(4) 0.2618(3) 0.141(6) Uani 1 1 d . U . . .
O91 O 0.4871(7) 0.3032(6) 0.2825(5) 0.204(11) Uani 1 1 d . U . . .
O92 O 0.5162(5) 0.3629(6) 0.2806(4) 0.179(9) Uani 1 1 d . U . . .
O93 O 0.6666(5) 0.3714(5) 0.1906(4) 0.166(8) Uani 1 1 d . U . . .
O94 O 0.6655(5) 0.4172(5) 0.2069(3) 0.154(7) Uani 1 1 d . U . . .
O95 O 0.6255(4) 0.4417(4) 0.2372(4) 0.144(6) Uani 1 1 d . U . . .
O96 O 0.5737(5) 0.4222(5) 0.2623(3) 0.150(7) Uani 1 1 d . U . . .
O97 O 0.5540(5) 0.4239(5) 0.3147(4) 0.169(9) Uani 1 1 d . . . . .
O98 O 0.5721(5) 0.4421(5) 0.3527(4) 0.173(9) Uani 1 1 d . U . . .
O99 O 0.6634(11) 0.4804(8) 0.0868(7) 0.075(9) Uiso 0.3 1 d . . P . .
O100 O 0.6761(8) 0.3896(8) 0.0831(7) 0.083(11) Uiso 0.3 1 d . . P . .
O101 O 0.4667(12) 0.4667(12) 0.250000 0.087(15) Uiso 0.3 2 d S . P . .
O102 O 0.4428(11) 0.4142(11) 0.1953(8) 0.063(11) Uiso 0.2 1 d . . P . .
O104 O 0.6915(7) 0.6647(7) 0.2520(5) 0.065(7) Uiso 0.3 1 d . . P . .
O107 O 0.6333(5) 0.6333(5) 0.250000 0.059(6) Uiso 0.5 2 d S . P . .
Se1 Se 0.59484(5) 0.44319(5) 0.24083(3) 0.0879(5) Uani 1 1 d . . . . .
Se2 Se 0.48545(5) 0.21959(5) 0.24080(3) 0.0878(5) Uani 1 1 d . . . . .
Se3 Se 0.55130(5) 0.44199(5) 0.33309(4) 0.0918(5) Uani 1 1 d . . . . .
Se4 Se 0.48382(6) 0.33171(6) 0.27597(4) 0.1012(6) Uani 1 1 d . . . . .
Se5 Se 0.66585(6) 0.40266(6) 0.18415(4) 0.1028(6) Uani 1 1 d . . . . .
Mo1 Mo 0.63564(2) 0.41063(2) 0.13340(2) 0.0508(2) Uani 1 1 d . . . . .
Mo2 Mo 0.43043(2) 0.33003(3) 0.23652(2) 0.0543(2) Uani 1 1 d . . . . .
Mo3 Mo 0.41451(2) 0.15649(2) 0.22165(2) 0.0544(2) Uani 1 1 d . . . . .
Mo4 Mo 0.41196(2) 0.32977(3) 0.27642(2) 0.0550(2) Uani 1 1 d . . . . .
Mo5 Mo 0.56380(3) 0.40351(3) 0.15788(2) 0.0505(3) Uani 0.9 1 d . . P . .
Mo6 Mo 0.76624(3) 0.50662(3) 0.15823(2) 0.0566(2) Uani 1 1 d . . . . .
Mo7 Mo 0.59148(3) 0.53785(3) 0.27820(2) 0.0575(3) Uani 1 1 d . . . . .
Mo8 Mo 0.66378(3) 0.56625(3) 0.24154(2) 0.0598(3) Uani 1 1 d . . . . .
Mo9 Mo 0.70786(3) 0.61213(3) 0.33736(2) 0.0537(3) Uani 0.9 1 d . . P . .
Mo10 Mo 0.49171(3) 0.37539(3) 0.19464(2) 0.0534(3) Uani 0.9 1 d . . P . .
Mo11 Mo 0.38792(3) 0.12307(3) 0.27793(2) 0.0544(3) Uani 0.9 1 d . . P . .
Mo12 Mo 0.44820(3) 0.28600(3) 0.19489(2) 0.0560(3) Uani 0.9 1 d . . P . .
Mo13 Mo 0.61839(4) 0.56533(4) 0.33745(2) 0.0559(3) Uani 0.8 1 d . . P . .
Mo14 Mo 0.56471(4) 0.33196(4) 0.13562(3) 0.0532(3) Uani 0.7 1 d . . P . .
Mo15 Mo 0.51017(2) 0.33134(2) 0.16587(2) 0.0508(2) Uani 1 1 d . . . . .
Mo16 Mo 0.69539(2) 0.44111(2) 0.13337(2) 0.0515(2) Uani 1 1 d . . . . .
Mo17 Mo 0.66333(3) 0.58203(2) 0.29399(2) 0.0525(2) Uani 1 1 d . . . . .
Mo18 Mo 0.53756(3) 0.50460(3) 0.32594(2) 0.0536(2) Uani 1 1 d . . . . .
Mo19 Mo 0.55629(3) 0.45707(2) 0.19709(2) 0.0530(2) Uani 1 1 d . . . . .
Mo20 Mo 0.48917(3) 0.45620(3) 0.34108(2) 0.0543(2) Uani 1 1 d . . . . .
Mo21 Mo 0.58585(3) 0.50549(2) 0.22183(2) 0.0534(2) Uani 1 1 d . . . . .
Mo22 Mo 0.43243(2) 0.20481(3) 0.19697(2) 0.0544(2) Uani 1 1 d . . . . .
Mo23 Mo 0.4024(3) 0.1369(3) 0.28040(16) 0.045(2) Uiso 0.1 1 d . . P . .
Mo24 Mo 0.57248(8) 0.33242(7) 0.14619(6) 0.0452(6) Uiso 0.3 1 d . . P . .
Mo25 Mo 0.62153(12) 0.55441(13) 0.33819(8) 0.0442(11) Uiso 0.2 1 d . . P . .
Mo26 Mo 0.4590(2) 0.28880(18) 0.20326(15) 0.0331(15) Uiso 0.1 1 d . . P . .
Mo27 Mo 0.4990(2) 0.3725(2) 0.20240(18) 0.042(2) Uiso 0.1 1 d . . P . .
Mo28 Mo 0.5681(3) 0.4028(3) 0.1644(2) 0.043(3) Uiso 0.1 1 d . . P . .
Mo29 Mo 0.7052(3) 0.5992(3) 0.33812(19) 0.050(3) Uiso 0.1 1 d . . P . .
Cl1 Cl 0.25024(17) 0.0041(2) 0.2494(2) 0.0719(18) Uiso 0.5 1 d . . P . .
O105 O 0.4661(19) 0.4294(19) 0.1112(14) 0.11(2) Uiso 0.2 1 d . . P A 1
N14 N 0.4545(13) 0.4130(14) 0.1241(9) 0.094(15) Uiso 0.3 1 d . . P B 2
H14A H 0.437699 0.398211 0.118088 0.113 Uiso 0.3 1 calc R U P B 2
H14B H 0.455344 0.430203 0.128062 0.113 Uiso 0.3 1 calc R U P B 2
C5 C 0.4798(10) 0.4090(10) 0.1275(7) 0.060(10) Uiso 0.3 1 d . . P B 2
N11 N 0.4797(9) 0.3853(9) 0.1223(7) 0.066(9) Uiso 0.3 1 d . . P B 2
H11A H 0.494140 0.381874 0.127206 0.079 Uiso 0.3 1 calc R U P B 2
H11B H 0.465227 0.371881 0.113669 0.079 Uiso 0.3 1 calc R U P B 2
N13 N 0.5020(8) 0.4301(8) 0.1408(6) 0.059(8) Uiso 0.3 1 d . . P B 2
H13A H 0.516529 0.426924 0.145847 0.071 Uiso 0.3 1 calc R U P B 2
H13B H 0.501759 0.446930 0.144423 0.071 Uiso 0.3 1 calc R U P B 2


_geom_special_details            
;
 All esds (except the esd in the dihedral angle between two l.s. planes)
 are estimated using the full covariance matrix.  The cell esds are taken
 into account individually in the estimation of esds in distances, angles
 and torsion angles; correlations between esds in cell parameters are only
 used when they are defined by crystal symmetry.  An approximate (isotropic)
 treatment of cell esds is used for estimating esds involving l.s. planes.
;

loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
C1 N2 1.27(3) . ?
C1 N1 1.33(3) . ?
C1 N3 1.45(3) . ?
C2 N6 1.25(2) . ?
C2 N4 1.27(2) . ?
C2 N5 1.29(2) . ?
C3 N7 1.27(2) . ?
C3 N8 1.333(19) . ?
C3 N9 1.383(18) . ?
C4 N10 1.310(13) 2_655 ?
C4 N10 1.310(14) 3_665 ?
C4 N10 1.310(13) . ?
N1 H1A 0.8800 . ?
N1 H1B 0.8800 . ?
N2 H2A 0.8800 . ?
N2 H2B 0.8800 . ?
N3 H3A 0.8800 . ?
N3 H3B 0.8800 . ?
N4 H4A 0.8800 . ?
N4 H4B 0.8800 . ?
N5 H5A 0.8800 . ?
N5 H5B 0.8800 . ?
N6 H6A 0.8800 . ?
N6 H6B 0.8800 . ?
N7 H7A 0.8800 . ?
N7 H7B 0.8800 . ?
N8 H8A 0.8800 . ?
N8 H8B 0.8800 . ?
N9 H9A 0.8800 . ?
N9 H9B 0.8800 . ?
N10 H10A 0.8800 . ?
N10 H10B 0.8800 . ?
O1 Mo17 2.017(9) . ?
O1 Mo8 2.046(8) . ?
O1 Mo11 2.054(8) 3_665 ?
O1 Mo23 2.091(13) 3_665 ?
O2 Mo15 1.996(8) . ?
O2 Mo14 2.058(8) . ?
O2 Mo5 2.065(8) . ?
O2 Mo24 2.066(9) . ?
O2 Mo28 2.068(15) . ?
O3 Mo17 2.003(9) . ?
O3 Mo11 2.050(9) 3_665 ?
O3 Mo29 2.053(14) . ?
O3 Mo9 2.076(8) . ?
O3 Mo23 2.095(13) 3_665 ?
O4 Mo17 2.010(9) . ?
O4 Mo25 2.035(10) . ?
O4 Mo13 2.041(8) . ?
O4 Mo7 2.071(8) . ?
O5 Mo9 1.785(9) . ?
O5 Mo29 1.851(15) . ?
O5 Mo20 2.058(9) 32 ?
O6 Mo15 1.996(8) . ?
O6 Mo28 2.023(15) . ?
O6 Mo5 2.065(8) . ?
O6 Mo10 2.068(8) . ?
O6 Mo27 2.069(12) . ?
O7 Mo24 1.796(9) . ?
O7 Mo14 1.800(9) . ?
O7 Mo16 2.061(9) 2_655 ?
O8 Mo28 1.777(16) . ?
O8 Mo5 1.782(9) . ?
O8 Mo1 2.049(9) . ?
O9 Mo28 1.963(16) . ?
O9 Mo5 2.420(8) . ?
O10 Mo10 1.766(9) . ?
O10 Mo27 1.834(13) . ?
O10 Mo19 2.075(9) . ?
O11 Mo8 1.780(9) 2_655 ?
O11 Mo3 2.057(9) . ?
O12 Mo7 1.787(9) . ?
O12 Mo18 2.063(9) . ?
O13 Mo15 2.340(7) . ?
O14 Mo13 1.787(10) . ?
O14 Mo25 1.851(11) . ?
O14 Mo18 2.031(10) . ?
O15 Mo24 1.688(9) . ?
O15 Mo14 2.434(9) . ?
O16 Mo8 1.772(9) . ?
O16 Mo21 2.074(9) . ?
O17 Mo7 2.430(9) . ?
O18 Mo23 1.718(15) . ?
O18 Mo11 2.438(9) . ?
O19 Mo4 1.935(9) . ?
O19 Mo2 1.955(9) . ?
O20 Mo6 1.804(9) 2_655 ?
O20 Mo22 2.037(9) . ?
O21 Mo23 1.759(13) 32 ?
O21 Mo11 1.782(9) 32 ?
O21 Mo20 2.065(9) . ?
O22 Mo17 2.328(8) . ?
O23 Mo25 1.770(10) . ?
O23 Mo13 1.789(9) . ?
O23 Mo4 2.057(9) 32 ?
O24 Mo6 1.794(8) . ?
O24 Mo16 2.045(8) . ?
O25 Mo4 1.933(10) . ?
O25 Mo2 1.935(9) . ?
O26 Mo19 1.950(9) . ?
O26 Mo21 1.966(9) . ?
O27 Mo29 1.778(15) . ?
O27 Mo9 1.797(9) . ?
O27 Mo4 2.073(9) 32 ?
O28 Mo14 1.664(9) . ?
O28 Mo24 2.413(10) . ?
O29 Mo16 1.679(9) . ?
O30 Mo29 1.791(16) . ?
O30 Mo9 2.385(8) . ?
O31 Mo6 2.405(8) . ?
O32 Mo26 1.682(13) . ?
O32 Mo12 2.385(9) . ?
O33 Mo12 1.785(9) . ?
O33 Mo26 1.852(12) . ?
O33 Mo22 2.050(9) . ?
O34 Mo23 1.799(13) . ?
O34 Mo11 1.806(9) . ?
O34 Mo3 2.041(9) . ?
O35 Mo7 1.693(10) . ?
O36 Mo3 1.922(9) . ?
O36 Mo22 1.958(8) . ?
O37 Mo1 1.662(8) . ?
O38 Mo12 1.705(10) . ?
O38 Mo26 2.407(14) . ?
O39 Mo17 1.683(9) . ?
O40 Mo9 1.675(9) . ?
O40 Mo29 2.266(17) . ?
O41 Mo13 1.651(10) . ?
O41 Mo25 2.289(11) . ?
O42 Mo5 1.660(9) . ?
O42 Mo28 2.121(16) . ?
O43 Mo6 1.689(9) . ?
O44 Mo8 1.685(9) . ?
O45 Mo10 1.662(9) . ?
O45 Mo27 2.314(15) . ?
O46 Mo20 1.685(9) . ?
O47 Mo2 1.697(10) . ?
O48 Mo19 1.677(9) . ?
O49 Mo18 1.636(8) . ?
O50 Mo11 1.685(9) . ?
O50 Mo23 2.412(16) . ?
O51 Se1 1.638(10) . ?
O51 Mo19 2.360(9) . ?
O52 Mo3 1.674(10) . ?
O53 Se5 1.608(10) . ?
O53 Mo1 2.351(9) . ?
O54 Se5 1.608(10) . ?
O54 Mo16 2.341(9) . ?
O55 Mo22 1.659(10) . ?
O56 Mo15 1.675(9) . ?
O57 Se2 1.647(10) . ?
O57 Mo22 2.354(10) . ?
O58 Mo4 1.662(9) . ?
O59 Se4 1.612(10) . ?
O59 Mo2 2.345(10) . ?
O60 Mo15 2.011(8) . ?
O60 Mo14 2.052(8) . ?
O60 Mo6 2.059(9) 2_655 ?
O60 Mo24 2.076(9) . ?
O61 Mo15 2.017(9) . ?
O61 Mo6 2.053(9) 2_655 ?
O61 Mo12 2.055(8) . ?
O61 Mo26 2.071(11) . ?
O62 Mo27 1.986(13) . ?
O62 Mo26 2.016(12) . ?
O62 Mo15 2.033(9) . ?
O62 Mo12 2.058(9) . ?
O62 Mo10 2.059(9) . ?
O63 Mo16 1.937(9) . ?
O63 Mo1 1.960(9) . ?
O64 Mo17 2.007(9) . ?
O64 Mo7 2.043(9) . ?
O64 Mo8 2.084(9) . ?
O65 Mo28 1.727(15) . ?
O65 Mo5 1.799(9) . ?
O65 Mo19 2.039(9) . ?
O66 Mo27 1.745(14) . ?
O66 Mo10 2.399(8) . ?
O67 Mo29 1.964(14) . ?
O67 Mo25 1.986(10) . ?
O67 Mo17 2.018(9) . ?
O67 Mo9 2.070(9) . ?
O67 Mo13 2.072(9) . ?
O68 Mo24 1.798(9) . ?
O68 Mo14 1.838(9) . ?
O68 Mo1 2.036(9) . ?
O69 Mo27 1.757(13) . ?
O69 Mo10 1.788(8) . ?
O69 Mo2 2.062(9) . ?
O70 Mo25 1.736(11) . ?
O70 Mo13 2.377(9) . ?
O71 Mo3 1.946(9) . ?
O71 Mo22 1.967(9) . ?
O72 Mo21 1.931(10) . ?
O72 Mo19 1.941(9) . ?
O73 Mo16 1.928(9) . ?
O73 Mo1 1.936(9) . ?
O74 Mo8 2.376(9) . ?
O75 Mo18 1.932(10) . ?
O75 Mo20 1.934(9) . ?
O76 Mo20 1.932(9) . ?
O76 Mo18 1.940(9) . ?
O77 Mo26 1.776(12) . ?
O77 Mo12 1.808(9) . ?
O77 Mo2 2.034(9) . ?
O78 Mo7 1.793(9) . ?
O78 Mo21 2.054(9) . ?
O79 Mo21 1.655(9) . ?
O80 Se3 1.619(10) . ?
O80 Mo18 2.367(10) . ?
O81 Se1 1.626(9) . ?
O81 Mo21 2.349(9) . ?
O82 Se2 1.633(9) . ?
O82 Mo3 2.366(9) . ?
O83 Se3 1.626(10) . ?
O83 Mo20 2.343(9) . ?
O84 Se4 1.629(10) . ?
O84 Mo4 2.363(9) . ?
O87 O88 0.98(3) 4 ?
O89 Se2 1.548(19) . ?
O90 Se2 1.578(19) . ?
O91 Se4 1.57(2) . ?
O92 Se4 1.63(2) . ?
O93 Se5 1.64(2) . ?
O94 Se5 1.57(2) . ?
O95 Se1 1.598(18) . ?
O96 Se1 1.69(2) . ?
O97 Se3 1.495(19) . ?
O98 Se3 1.59(2) . ?
O99 O99 0.52(8) 18_654 ?
O100 O100 0.82(7) 18_654 ?
Mo1 Mo16 2.6049(16) . ?
Mo2 Mo4 2.6068(16) . ?
Mo3 Mo22 2.6095(16) . ?
Mo9 Mo29 0.598(13) . ?
Mo10 Mo27 0.658(12) . ?
Mo11 Mo23 0.727(12) . ?
Mo12 Mo26 0.706(9) . ?
Mo13 Mo25 0.645(5) . ?
Mo14 Mo24 0.750(4) . ?
Mo18 Mo20 2.6060(17) . ?
Mo19 Mo21 2.6103(16) . ?
N14 C5 1.40(7) . ?
N14 H14A 0.8800 . ?
N14 H14B 0.8800 . ?
C5 N11 1.23(6) . ?
C5 N13 1.36(6) . ?
N11 H11A 0.8800 . ?
N11 H11B 0.8800 . ?
N13 H13A 0.8800 . ?
N13 H13B 0.8800 . ?

loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
N2 C1 N1 124(2) . . ?
N2 C1 N3 118(2) . . ?
N1 C1 N3 118(2) . . ?
N6 C2 N4 116.4(18) . . ?
N6 C2 N5 120.5(19) . . ?
N4 C2 N5 123.0(16) . . ?
N7 C3 N8 122.7(14) . . ?
N7 C3 N9 119.4(13) . . ?
N8 C3 N9 117.9(14) . . ?
N10 C4 N10 119.97(13) 2_655 3_665 ?
N10 C4 N10 119.96(13) 2_655 . ?
N10 C4 N10 119.97(13) 3_665 . ?
C1 N1 H1A 120.0 . . ?
C1 N1 H1B 120.0 . . ?
H1A N1 H1B 120.0 . . ?
C1 N2 H2A 120.0 . . ?
C1 N2 H2B 120.0 . . ?
H2A N2 H2B 120.0 . . ?
C1 N3 H3A 120.0 . . ?
C1 N3 H3B 120.0 . . ?
H3A N3 H3B 120.0 . . ?
C2 N4 H4A 120.0 . . ?
C2 N4 H4B 120.0 . . ?
H4A N4 H4B 120.0 . . ?
C2 N5 H5A 120.0 . . ?
C2 N5 H5B 120.0 . . ?
H5A N5 H5B 120.0 . . ?
C2 N6 H6A 120.0 . . ?
C2 N6 H6B 120.0 . . ?
H6A N6 H6B 120.0 . . ?
C3 N7 H7A 120.0 . . ?
C3 N7 H7B 120.0 . . ?
H7A N7 H7B 120.0 . . ?
C3 N8 H8A 120.0 . . ?
C3 N8 H8B 120.0 . . ?
H8A N8 H8B 120.0 . . ?
C3 N9 H9A 120.0 . . ?
C3 N9 H9B 120.0 . . ?
H9A N9 H9B 120.0 . . ?
C4 N10 H10A 120.0 . . ?
C4 N10 H10B 120.0 . . ?
H10A N10 H10B 120.0 . . ?
Mo17 O1 Mo8 108.8(4) . . ?
Mo17 O1 Mo11 108.0(4) . 3_665 ?
Mo8 O1 Mo11 140.4(4) . 3_665 ?
Mo17 O1 Mo23 110.0(5) . 3_665 ?
Mo8 O1 Mo23 140.7(5) . 3_665 ?
Mo11 O1 Mo23 20.2(3) 3_665 3_665 ?
Mo15 O2 Mo14 108.8(4) . . ?
Mo15 O2 Mo5 108.9(4) . . ?
Mo14 O2 Mo5 139.8(4) . . ?
Mo15 O2 Mo24 110.3(4) . . ?
Mo14 O2 Mo24 20.94(13) . . ?
Mo5 O2 Mo24 140.0(5) . . ?
Mo15 O2 Mo28 109.1(5) . . ?
Mo14 O2 Mo28 142.1(6) . . ?
Mo5 O2 Mo28 12.9(4) . . ?
Mo24 O2 Mo28 135.3(6) . . ?
Mo17 O3 Mo11 108.7(4) . 3_665 ?
Mo17 O3 Mo29 107.0(5) . . ?
Mo11 O3 Mo29 144.1(6) 3_665 . ?
Mo17 O3 Mo9 108.4(4) . . ?
Mo11 O3 Mo9 140.4(5) 3_665 . ?
Mo29 O3 Mo9 16.6(4) . . ?
Mo17 O3 Mo23 110.4(5) . 3_665 ?
Mo11 O3 Mo23 20.2(3) 3_665 3_665 ?
Mo29 O3 Mo23 135.5(6) . 3_665 ?
Mo9 O3 Mo23 140.6(5) . 3_665 ?
Mo17 O4 Mo25 108.1(4) . . ?
Mo17 O4 Mo13 109.7(4) . . ?
Mo25 O4 Mo13 18.21(17) . . ?
Mo17 O4 Mo7 108.1(4) . . ?
Mo25 O4 Mo7 143.0(5) . . ?
Mo13 O4 Mo7 140.6(5) . . ?
Mo9 O5 Mo29 18.8(4) . . ?
Mo9 O5 Mo20 156.0(5) . 32 ?
Mo29 O5 Mo20 150.0(6) . 32 ?
Mo15 O6 Mo28 110.9(5) . . ?
Mo15 O6 Mo5 108.9(4) . . ?
Mo28 O6 Mo5 12.9(4) . . ?
Mo15 O6 Mo10 108.9(4) . . ?
Mo28 O6 Mo10 140.2(6) . . ?
Mo5 O6 Mo10 139.9(4) . . ?
Mo15 O6 Mo27 107.6(5) . . ?
Mo28 O6 Mo27 137.1(6) . . ?
Mo5 O6 Mo27 143.1(5) . . ?
Mo10 O6 Mo27 18.3(3) . . ?
Mo24 O7 Mo14 24.07(16) . . ?
Mo24 O7 Mo16 149.7(5) . 2_655 ?
Mo14 O7 Mo16 155.7(5) . 2_655 ?
Mo28 O8 Mo5 14.9(4) . . ?
Mo28 O8 Mo1 155.2(7) . . ?
Mo5 O8 Mo1 158.1(5) . . ?
Mo28 O9 Mo5 1.9(4) . . ?
Mo10 O10 Mo27 21.0(4) . . ?
Mo10 O10 Mo19 156.2(5) . . ?
Mo27 O10 Mo19 149.9(6) . . ?
Mo8 O11 Mo3 156.2(5) 2_655 . ?
Mo7 O12 Mo18 155.1(5) . . ?
Mo13 O14 Mo25 20.3(2) . . ?
Mo13 O14 Mo18 156.1(5) . . ?
Mo25 O14 Mo18 150.9(5) . . ?
Mo24 O15 Mo14 2.07(15) . . ?
Mo8 O16 Mo21 156.7(5) . . ?
Mo23 O18 Mo11 2.9(3) . . ?
Mo4 O19 Mo2 84.1(4) . . ?
Mo6 O20 Mo22 156.8(5) 2_655 . ?
Mo23 O21 Mo11 23.7(4) 32 32 ?
Mo23 O21 Mo20 148.7(6) 32 . ?
Mo11 O21 Mo20 156.3(5) 32 . ?
Mo25 O23 Mo13 20.9(2) . . ?
Mo25 O23 Mo4 149.3(6) . 32 ?
Mo13 O23 Mo4 157.5(5) . 32 ?
Mo6 O24 Mo16 156.7(5) . . ?
Mo4 O25 Mo2 84.8(4) . . ?
Mo19 O26 Mo21 83.6(3) . . ?
Mo29 O27 Mo9 19.2(4) . . ?
Mo29 O27 Mo4 146.5(7) . 32 ?
Mo9 O27 Mo4 155.6(5) . 32 ?
Mo14 O28 Mo24 0.41(13) . . ?
Mo29 O30 Mo9 1.8(4) . . ?
Mo26 O32 Mo12 2.0(3) . . ?
Mo12 O33 Mo26 22.3(3) . . ?
Mo12 O33 Mo22 156.5(5) . . ?
Mo26 O33 Mo22 149.2(6) . . ?
Mo23 O34 Mo11 23.3(4) . . ?
Mo23 O34 Mo3 148.0(6) . . ?
Mo11 O34 Mo3 156.8(6) . . ?
Mo3 O36 Mo22 84.5(3) . . ?
Mo12 O38 Mo26 2.2(2) . . ?
Mo9 O40 Mo29 2.6(3) . . ?
Mo13 O41 Mo25 2.88(19) . . ?
Mo5 O42 Mo28 1.2(4) . . ?
Mo10 O45 Mo27 2.5(3) . . ?
Mo11 O50 Mo23 0.7(3) . . ?
Se1 O51 Mo19 125.6(5) . . ?
Se5 O53 Mo1 127.4(5) . . ?
Se5 O54 Mo16 128.1(6) . . ?
Se2 O57 Mo22 126.5(6) . . ?
Se4 O59 Mo2 128.6(5) . . ?
Mo15 O60 Mo14 108.5(4) . . ?
Mo15 O60 Mo6 108.5(4) . 2_655 ?
Mo14 O60 Mo6 140.6(4) . 2_655 ?
Mo15 O60 Mo24 109.3(4) . . ?
Mo14 O60 Mo24 20.91(13) . . ?
Mo6 O60 Mo24 141.3(4) 2_655 . ?
Mo15 O61 Mo6 108.5(4) . 2_655 ?
Mo15 O61 Mo12 108.8(4) . . ?
Mo6 O61 Mo12 140.7(5) 2_655 . ?
Mo15 O61 Mo26 107.9(5) . . ?
Mo6 O61 Mo26 142.7(5) 2_655 . ?
Mo12 O61 Mo26 19.7(3) . . ?
Mo27 O62 Mo26 131.7(6) . . ?
Mo27 O62 Mo15 109.4(5) . . ?
Mo26 O62 Mo15 109.5(5) . . ?
Mo27 O62 Mo12 141.6(5) . . ?
Mo26 O62 Mo12 19.9(3) . . ?
Mo15 O62 Mo12 108.1(4) . . ?
Mo27 O62 Mo10 18.6(3) . . ?
Mo26 O62 Mo10 141.6(5) . . ?
Mo15 O62 Mo10 107.8(4) . . ?
Mo12 O62 Mo10 142.4(5) . . ?
Mo16 O63 Mo1 83.9(3) . . ?
Mo17 O64 Mo7 109.3(4) . . ?
Mo17 O64 Mo8 107.7(4) . . ?
Mo7 O64 Mo8 140.7(4) . . ?
Mo28 O65 Mo5 14.9(4) . . ?
Mo28 O65 Mo19 153.1(7) . . ?
Mo5 O65 Mo19 157.3(5) . . ?
Mo27 O66 Mo10 2.2(4) . . ?
Mo29 O67 Mo25 135.0(6) . . ?
Mo29 O67 Mo17 110.0(5) . . ?
Mo25 O67 Mo17 109.8(4) . . ?
Mo29 O67 Mo9 16.8(4) . . ?
Mo25 O67 Mo9 142.0(5) . . ?
Mo17 O67 Mo9 108.1(4) . . ?
Mo29 O67 Mo13 141.8(6) . . ?
Mo25 O67 Mo13 18.13(18) . . ?
Mo17 O67 Mo13 108.2(4) . . ?
Mo9 O67 Mo13 140.8(5) . . ?
Mo24 O68 Mo14 23.77(16) . . ?
Mo24 O68 Mo1 149.8(5) . . ?
Mo14 O68 Mo1 155.1(5) . . ?
Mo27 O69 Mo10 21.4(4) . . ?
Mo27 O69 Mo2 147.6(6) . . ?
Mo10 O69 Mo2 157.0(5) . . ?
Mo25 O70 Mo13 2.0(2) . . ?
Mo3 O71 Mo22 83.6(4) . . ?
Mo21 O72 Mo19 84.8(4) . . ?
Mo16 O73 Mo1 84.8(4) . . ?
Mo18 O75 Mo20 84.8(4) . . ?
Mo20 O76 Mo18 84.6(3) . . ?
Mo26 O77 Mo12 22.7(3) . . ?
Mo26 O77 Mo2 148.9(6) . . ?
Mo12 O77 Mo2 156.7(5) . . ?
Mo7 O78 Mo21 155.5(6) . . ?
Se3 O80 Mo18 126.5(5) . . ?
Se1 O81 Mo21 127.4(6) . . ?
Se2 O82 Mo3 126.6(5) . . ?
Se3 O83 Mo20 127.4(6) . . ?
Se4 O84 Mo4 125.8(5) . . ?
O95 Se1 O81 110.1(8) . . ?
O95 Se1 O51 109.1(8) . . ?
O81 Se1 O51 106.7(5) . . ?
O95 Se1 O96 113.5(11) . . ?
O81 Se1 O96 110.0(8) . . ?
O51 Se1 O96 107.1(8) . . ?
O89 Se2 O90 111.9(13) . . ?
O89 Se2 O82 110.5(9) . . ?
O90 Se2 O82 108.5(8) . . ?
O89 Se2 O57 108.9(10) . . ?
O90 Se2 O57 110.4(8) . . ?
O82 Se2 O57 106.5(5) . . ?
O97 Se3 O98 107.9(15) . . ?
O97 Se3 O80 109.8(10) . . ?
O98 Se3 O80 107.8(9) . . ?
O97 Se3 O83 112.6(9) . . ?
O98 Se3 O83 112.4(10) . . ?
O80 Se3 O83 106.3(5) . . ?
O91 Se4 O59 112.9(12) . . ?
O91 Se4 O92 108.8(15) . . ?
O59 Se4 O92 109.5(10) . . ?
O91 Se4 O84 110.5(12) . . ?
O59 Se4 O84 106.0(5) . . ?
O92 Se4 O84 109.1(10) . . ?
O94 Se5 O53 111.2(9) . . ?
O94 Se5 O54 111.7(10) . . ?
O53 Se5 O54 105.3(5) . . ?
O94 Se5 O93 104.1(13) . . ?
O53 Se5 O93 112.5(9) . . ?
O54 Se5 O93 112.2(9) . . ?
O37 Mo1 O73 103.7(4) . . ?
O37 Mo1 O63 104.8(4) . . ?
O73 Mo1 O63 93.1(4) . . ?
O37 Mo1 O68 96.3(4) . . ?
O73 Mo1 O68 159.3(3) . . ?
O63 Mo1 O68 86.6(4) . . ?
O37 Mo1 O8 95.8(4) . . ?
O73 Mo1 O8 89.4(4) . . ?
O63 Mo1 O8 157.9(4) . . ?
O68 Mo1 O8 83.4(3) . . ?
O37 Mo1 O53 170.7(4) . . ?
O73 Mo1 O53 82.2(4) . . ?
O63 Mo1 O53 81.7(4) . . ?
O68 Mo1 O53 77.3(4) . . ?
O8 Mo1 O53 76.9(3) . . ?
O37 Mo1 Mo16 99.8(3) . . ?
O73 Mo1 Mo16 47.5(3) . . ?
O63 Mo1 Mo16 47.7(3) . . ?
O68 Mo1 Mo16 134.0(2) . . ?
O8 Mo1 Mo16 136.5(2) . . ?
O53 Mo1 Mo16 89.5(2) . . ?
O47 Mo2 O25 104.2(5) . . ?
O47 Mo2 O19 103.6(5) . . ?
O25 Mo2 O19 93.2(4) . . ?
O47 Mo2 O77 96.2(5) . . ?
O25 Mo2 O77 158.8(4) . . ?
O19 Mo2 O77 87.2(4) . . ?
O47 Mo2 O69 97.6(4) . . ?
O25 Mo2 O69 88.1(4) . . ?
O19 Mo2 O69 157.8(3) . . ?
O77 Mo2 O69 83.8(3) . . ?
O47 Mo2 O59 171.5(4) . . ?
O25 Mo2 O59 82.7(4) . . ?
O19 Mo2 O59 80.6(4) . . ?
O77 Mo2 O59 76.5(4) . . ?
O69 Mo2 O59 77.5(4) . . ?
O47 Mo2 Mo4 99.3(4) . . ?
O25 Mo2 Mo4 47.6(3) . . ?
O19 Mo2 Mo4 47.6(3) . . ?
O77 Mo2 Mo4 134.5(3) . . ?
O69 Mo2 Mo4 135.3(2) . . ?
O59 Mo2 Mo4 89.0(2) . . ?
O52 Mo3 O36 104.5(5) . . ?
O52 Mo3 O71 104.7(4) . . ?
O36 Mo3 O71 94.5(4) . . ?
O52 Mo3 O34 95.1(4) . . ?
O36 Mo3 O34 87.7(4) . . ?
O71 Mo3 O34 158.8(4) . . ?
O52 Mo3 O11 96.5(5) . . ?
O36 Mo3 O11 157.8(4) . . ?
O71 Mo3 O11 86.6(4) . . ?
O34 Mo3 O11 83.6(4) . . ?
O52 Mo3 O82 170.2(4) . . ?
O36 Mo3 O82 82.3(4) . . ?
O71 Mo3 O82 81.4(4) . . ?
O34 Mo3 O82 78.0(4) . . ?
O11 Mo3 O82 76.0(3) . . ?
O52 Mo3 Mo22 99.7(4) . . ?
O36 Mo3 Mo22 48.3(3) . . ?
O71 Mo3 Mo22 48.5(3) . . ?
O34 Mo3 Mo22 135.8(3) . . ?
O11 Mo3 Mo22 134.8(2) . . ?
O82 Mo3 Mo22 90.1(2) . . ?
O58 Mo4 O25 103.5(5) . . ?
O58 Mo4 O19 103.5(5) . . ?
O25 Mo4 O19 93.8(4) . . ?
O58 Mo4 O23 96.7(4) . 33_545 ?
O25 Mo4 O23 158.9(4) . 33_545 ?
O19 Mo4 O23 87.2(4) . 33_545 ?
O58 Mo4 O27 96.5(4) . 33_545 ?
O25 Mo4 O27 87.9(4) . 33_545 ?
O19 Mo4 O27 158.9(4) . 33_545 ?
O23 Mo4 O27 83.8(4) 33_545 33_545 ?
O58 Mo4 O84 170.8(4) . . ?
O25 Mo4 O84 82.4(4) . . ?
O19 Mo4 O84 82.9(4) . . ?
O23 Mo4 O84 76.8(4) 33_545 . ?
O27 Mo4 O84 76.5(4) 33_545 . ?
O58 Mo4 Mo2 98.7(3) . . ?
O25 Mo4 Mo2 47.7(3) . . ?
O19 Mo4 Mo2 48.2(3) . . ?
O23 Mo4 Mo2 135.1(3) 33_545 . ?
O27 Mo4 Mo2 135.3(3) 33_545 . ?
O84 Mo4 Mo2 90.5(3) . . ?
O42 Mo5 O8 103.3(5) . . ?
O42 Mo5 O65 103.5(4) . . ?
O8 Mo5 O65 105.5(4) . . ?
O42 Mo5 O2 97.0(4) . . ?
O8 Mo5 O2 89.0(4) . . ?
O65 Mo5 O2 151.0(4) . . ?
O42 Mo5 O6 97.2(4) . . ?
O8 Mo5 O6 151.1(4) . . ?
O65 Mo5 O6 88.9(4) . . ?
O2 Mo5 O6 68.3(3) . . ?
O42 Mo5 O9 172.5(4) . . ?
O8 Mo5 O9 80.3(4) . . ?
O65 Mo5 O9 81.6(3) . . ?
O2 Mo5 O9 76.2(3) . . ?
O6 Mo5 O9 77.3(3) . . ?
O43 Mo6 O24 103.0(4) . . ?
O43 Mo6 O20 103.3(5) . 3_665 ?
O24 Mo6 O20 104.5(4) . 3_665 ?
O43 Mo6 O61 96.9(4) . 3_665 ?
O24 Mo6 O61 152.5(4) . 3_665 ?
O20 Mo6 O61 88.9(4) 3_665 3_665 ?
O43 Mo6 O60 97.4(4) . 3_665 ?
O24 Mo6 O60 89.3(4) . 3_665 ?
O20 Mo6 O60 151.6(4) 3_665 3_665 ?
O61 Mo6 O60 69.3(3) 3_665 3_665 ?
O43 Mo6 O31 173.0(4) . . ?
O24 Mo6 O31 81.0(3) . . ?
O20 Mo6 O31 81.0(4) 3_665 . ?
O61 Mo6 O31 77.5(3) 3_665 . ?
O60 Mo6 O31 76.8(3) 3_665 . ?
O35 Mo7 O12 102.8(5) . . ?
O35 Mo7 O78 103.1(4) . . ?
O12 Mo7 O78 103.5(4) . . ?
O35 Mo7 O64 97.5(5) . . ?
O12 Mo7 O64 152.4(4) . . ?
O78 Mo7 O64 89.7(4) . . ?
O35 Mo7 O4 96.8(4) . . ?
O12 Mo7 O4 89.9(4) . . ?
O78 Mo7 O4 152.7(4) . . ?
O64 Mo7 O4 69.1(3) . . ?
O35 Mo7 O17 174.1(5) . . ?
O12 Mo7 O17 80.9(4) . . ?
O78 Mo7 O17 80.1(4) . . ?
O64 Mo7 O17 77.6(3) . . ?
O4 Mo7 O17 78.6(3) . . ?
O44 Mo8 O16 102.8(4) . . ?
O44 Mo8 O11 102.6(4) . 3_665 ?
O16 Mo8 O11 105.0(4) . 3_665 ?
O44 Mo8 O1 95.7(4) . . ?
O16 Mo8 O1 152.9(4) . . ?
O11 Mo8 O1 89.8(4) 3_665 . ?
O44 Mo8 O64 96.1(4) . . ?
O16 Mo8 O64 89.1(4) . . ?
O11 Mo8 O64 153.2(4) 3_665 . ?
O1 Mo8 O64 69.3(3) . . ?
O44 Mo8 O74 172.3(4) . . ?
O16 Mo8 O74 82.2(4) . . ?
O11 Mo8 O74 81.5(4) 3_665 . ?
O1 Mo8 O74 77.6(3) . . ?
O64 Mo8 O74 78.0(3) . . ?
Mo29 Mo9 O40 170.1(13) . . ?
Mo29 Mo9 O5 86.8(12) . . ?
O40 Mo9 O5 102.3(5) . . ?
Mo29 Mo9 O27 78.6(12) . . ?
O40 Mo9 O27 102.4(4) . . ?
O5 Mo9 O27 104.7(4) . . ?
Mo29 Mo9 O67 71.5(12) . . ?
O40 Mo9 O67 98.6(4) . . ?
O5 Mo9 O67 151.5(4) . . ?
O27 Mo9 O67 89.4(4) . . ?
Mo29 Mo9 O3 79.5(12) . . ?
O40 Mo9 O3 96.7(4) . . ?
O5 Mo9 O3 89.4(4) . . ?
O27 Mo9 O3 153.1(4) . . ?
O67 Mo9 O3 68.9(3) . . ?
Mo29 Mo9 O30 5.5(12) . . ?
O40 Mo9 O30 173.4(4) . . ?
O5 Mo9 O30 81.6(3) . . ?
O27 Mo9 O30 81.5(4) . . ?
O67 Mo9 O30 76.0(3) . . ?
O3 Mo9 O30 78.0(3) . . ?
Mo27 Mo10 O45 171.2(9) . . ?
Mo27 Mo10 O10 85.4(9) . . ?
O45 Mo10 O10 103.1(5) . . ?
Mo27 Mo10 O69 76.7(9) . . ?
O45 Mo10 O69 103.1(4) . . ?
O10 Mo10 O69 104.9(4) . . ?
Mo27 Mo10 O62 74.4(9) . . ?
O45 Mo10 O62 96.7(4) . . ?
O10 Mo10 O62 152.7(4) . . ?
O69 Mo10 O62 88.3(4) . . ?
Mo27 Mo10 O6 80.9(9) . . ?
O45 Mo10 O6 96.5(4) . . ?
O10 Mo10 O6 89.8(4) . . ?
O69 Mo10 O6 151.9(3) . . ?
O62 Mo10 O6 69.4(3) . . ?
Mo27 Mo10 O66 5.8(9) . . ?
O45 Mo10 O66 173.0(4) . . ?
O10 Mo10 O66 80.7(3) . . ?
O69 Mo10 O66 81.3(3) . . ?
O62 Mo10 O66 77.9(3) . . ?
O6 Mo10 O66 77.6(3) . . ?
Mo23 Mo11 O50 177.7(9) . . ?
Mo23 Mo11 O21 76.4(8) . 33_545 ?
O50 Mo11 O21 101.7(4) . 33_545 ?
Mo23 Mo11 O34 77.9(8) . . ?
O50 Mo11 O34 101.6(4) . . ?
O21 Mo11 O34 104.7(4) 33_545 . ?
Mo23 Mo11 O3 83.4(8) . 2_655 ?
O50 Mo11 O3 97.9(4) . 2_655 ?
O21 Mo11 O3 89.3(4) 33_545 2_655 ?
O34 Mo11 O3 153.0(4) . 2_655 ?
Mo23 Mo11 O1 82.7(8) . 2_655 ?
O50 Mo11 O1 99.5(4) . 2_655 ?
O21 Mo11 O1 151.7(4) 33_545 2_655 ?
O34 Mo11 O1 89.1(4) . 2_655 ?
O3 Mo11 O1 69.3(3) 2_655 2_655 ?
Mo23 Mo11 O18 6.9(8) . . ?
O50 Mo11 O18 175.2(4) . . ?
O21 Mo11 O18 81.0(4) 33_545 . ?
O34 Mo11 O18 81.5(4) . . ?
O3 Mo11 O18 78.1(3) 2_655 . ?
O1 Mo11 O18 76.8(3) 2_655 . ?
Mo26 Mo12 O38 172.5(8) . . ?
Mo26 Mo12 O33 84.2(7) . . ?
O38 Mo12 O33 103.3(5) . . ?
Mo26 Mo12 O77 76.1(7) . . ?
O38 Mo12 O77 102.7(4) . . ?
O33 Mo12 O77 105.0(4) . . ?
Mo26 Mo12 O61 81.5(7) . . ?
O38 Mo12 O61 97.3(4) . . ?
O33 Mo12 O61 89.5(4) . . ?
O77 Mo12 O61 151.6(4) . . ?
Mo26 Mo12 O62 76.7(7) . . ?
O38 Mo12 O62 95.9(4) . . ?
O33 Mo12 O62 153.5(4) . . ?
O77 Mo12 O62 88.2(4) . . ?
O61 Mo12 O62 69.8(4) . . ?
Mo26 Mo12 O32 4.7(7) . . ?
O38 Mo12 O32 173.7(4) . . ?
O33 Mo12 O32 81.0(4) . . ?
O77 Mo12 O32 80.3(4) . . ?
O61 Mo12 O32 78.0(3) . . ?
O62 Mo12 O32 78.7(3) . . ?
Mo25 Mo13 O41 169.7(7) . . ?
Mo25 Mo13 O14 85.4(6) . . ?
O41 Mo13 O14 104.6(5) . . ?
Mo25 Mo13 O23 77.9(6) . . ?
O41 Mo13 O23 101.4(5) . . ?
O14 Mo13 O23 105.2(4) . . ?
Mo25 Mo13 O4 80.3(5) . . ?
O41 Mo13 O4 96.9(4) . . ?
O14 Mo13 O4 89.9(4) . . ?
O23 Mo13 O4 152.2(4) . . ?
Mo25 Mo13 O67 73.3(5) . . ?
O41 Mo13 O67 96.5(5) . . ?
O14 Mo13 O67 151.9(4) . . ?
O23 Mo13 O67 88.3(4) . . ?
O4 Mo13 O67 68.9(3) . . ?
Mo25 Mo13 O70 5.4(5) . . ?
O41 Mo13 O70 173.4(5) . . ?
O14 Mo13 O70 80.4(4) . . ?
O23 Mo13 O70 81.2(4) . . ?
O4 Mo13 O70 78.5(3) . . ?
O67 Mo13 O70 77.5(3) . . ?
Mo24 Mo14 O28 178.7(4) . . ?
Mo24 Mo14 O7 77.6(4) . . ?
O28 Mo14 O7 103.5(4) . . ?
Mo24 Mo14 O68 75.1(4) . . ?
O28 Mo14 O68 103.9(4) . . ?
O7 Mo14 O68 103.0(4) . . ?
Mo24 Mo14 O60 81.4(4) . . ?
O28 Mo14 O60 99.3(4) . . ?
O7 Mo14 O60 89.1(4) . . ?
O68 Mo14 O60 150.4(4) . . ?
Mo24 Mo14 O2 80.1(4) . . ?
O28 Mo14 O2 99.1(4) . . ?
O7 Mo14 O2 150.7(4) . . ?
O68 Mo14 O2 89.3(4) . . ?
O60 Mo14 O2 68.9(3) . . ?
Mo24 Mo14 O15 4.7(3) . . ?
O28 Mo14 O15 175.6(4) . . ?
O7 Mo14 O15 78.7(4) . . ?
O68 Mo14 O15 79.1(4) . . ?
O60 Mo14 O15 76.8(3) . . ?
O2 Mo14 O15 77.6(3) . . ?
O56 Mo15 O6 99.1(4) . . ?
O56 Mo15 O2 99.3(4) . . ?
O6 Mo15 O2 71.0(3) . . ?
O56 Mo15 O60 98.9(4) . . ?
O6 Mo15 O60 139.9(3) . . ?
O2 Mo15 O60 70.9(3) . . ?
O56 Mo15 O61 98.3(4) . . ?
O6 Mo15 O61 140.3(3) . . ?
O2 Mo15 O61 139.9(3) . . ?
O60 Mo15 O61 71.0(3) . . ?
O56 Mo15 O62 98.1(4) . . ?
O6 Mo15 O62 71.4(3) . . ?
O2 Mo15 O62 140.4(3) . . ?
O60 Mo15 O62 140.1(3) . . ?
O61 Mo15 O62 71.0(3) . . ?
O56 Mo15 O13 179.8(6) . . ?
O6 Mo15 O13 81.0(3) . . ?
O2 Mo15 O13 80.9(3) . . ?
O60 Mo15 O13 81.2(3) . . ?
O61 Mo15 O13 81.6(3) . . ?
O62 Mo15 O13 81.7(3) . . ?
O29 Mo16 O73 103.8(5) . . ?
O29 Mo16 O63 104.9(4) . . ?
O73 Mo16 O63 94.1(4) . . ?
O29 Mo16 O24 96.2(4) . . ?
O73 Mo16 O24 88.4(4) . . ?
O63 Mo16 O24 157.5(4) . . ?
O29 Mo16 O7 95.8(4) . 3_665 ?
O73 Mo16 O7 159.5(4) . 3_665 ?
O63 Mo16 O7 86.3(4) . 3_665 ?
O24 Mo16 O7 83.8(3) . 3_665 ?
O29 Mo16 O54 170.8(4) . . ?
O73 Mo16 O54 81.9(4) . . ?
O63 Mo16 O54 81.6(4) . . ?
O24 Mo16 O54 76.7(4) . . ?
O7 Mo16 O54 77.9(4) 3_665 . ?
O29 Mo16 Mo1 99.9(3) . . ?
O73 Mo16 Mo1 47.7(3) . . ?
O63 Mo16 Mo1 48.4(3) . . ?
O24 Mo16 Mo1 135.7(2) . . ?
O7 Mo16 Mo1 134.5(3) 3_665 . ?
O54 Mo16 Mo1 89.3(3) . . ?
O39 Mo17 O3 99.0(4) . . ?
O39 Mo17 O64 98.8(4) . . ?
O3 Mo17 O64 140.4(3) . . ?
O39 Mo17 O4 97.2(4) . . ?
O3 Mo17 O4 140.4(3) . . ?
O64 Mo17 O4 71.0(3) . . ?
O39 Mo17 O1 99.8(4) . . ?
O3 Mo17 O1 70.9(3) . . ?
O64 Mo17 O1 71.3(3) . . ?
O4 Mo17 O1 140.5(3) . . ?
O39 Mo17 O67 98.7(4) . . ?
O3 Mo17 O67 71.4(3) . . ?
O64 Mo17 O67 139.3(4) . . ?
O4 Mo17 O67 70.6(3) . . ?
O1 Mo17 O67 140.0(3) . . ?
O39 Mo17 O22 179.2(4) . . ?
O3 Mo17 O22 81.7(3) . . ?
O64 Mo17 O22 80.9(3) . . ?
O4 Mo17 O22 82.1(3) . . ?
O1 Mo17 O22 80.7(3) . . ?
O67 Mo17 O22 81.2(3) . . ?
O49 Mo18 O75 104.1(5) . . ?
O49 Mo18 O76 104.7(4) . . ?
O75 Mo18 O76 92.8(4) . . ?
O49 Mo18 O14 97.0(5) . . ?
O75 Mo18 O14 158.0(4) . . ?
O76 Mo18 O14 87.7(4) . . ?
O49 Mo18 O12 96.3(4) . . ?
O75 Mo18 O12 87.0(4) . . ?
O76 Mo18 O12 158.3(4) . . ?
O14 Mo18 O12 84.7(3) . . ?
O49 Mo18 O80 171.0(4) . . ?
O75 Mo18 O80 81.1(4) . . ?
O76 Mo18 O80 82.1(4) . . ?
O14 Mo18 O80 77.2(4) . . ?
O12 Mo18 O80 76.4(4) . . ?
O49 Mo18 Mo20 99.0(4) . . ?
O75 Mo18 Mo20 47.7(3) . . ?
O76 Mo18 Mo20 47.6(3) . . ?
O14 Mo18 Mo20 134.9(2) . . ?
O12 Mo18 Mo20 134.4(3) . . ?
O80 Mo18 Mo20 89.9(3) . . ?
O48 Mo19 O72 104.3(4) . . ?
O48 Mo19 O26 105.7(4) . . ?
O72 Mo19 O26 93.5(4) . . ?
O48 Mo19 O65 96.1(4) . . ?
O72 Mo19 O65 158.5(4) . . ?
O26 Mo19 O65 87.4(4) . . ?
O48 Mo19 O10 94.6(4) . . ?
O72 Mo19 O10 87.9(4) . . ?
O26 Mo19 O10 158.6(3) . . ?
O65 Mo19 O10 83.6(3) . . ?
O48 Mo19 O51 169.3(4) . . ?
O72 Mo19 O51 82.0(4) . . ?
O26 Mo19 O51 82.3(4) . . ?
O65 Mo19 O51 76.8(4) . . ?
O10 Mo19 O51 76.7(4) . . ?
O48 Mo19 Mo21 100.0(4) . . ?
O72 Mo19 Mo21 47.4(3) . . ?
O26 Mo19 Mo21 48.5(3) . . ?
O65 Mo19 Mo21 135.7(3) . . ?
O10 Mo19 Mo21 135.1(2) . . ?
O51 Mo19 Mo21 90.6(3) . . ?
O46 Mo20 O76 104.9(4) . . ?
O46 Mo20 O75 104.5(4) . . ?
O76 Mo20 O75 93.0(4) . . ?
O46 Mo20 O5 95.9(4) . 33_545 ?
O76 Mo20 O5 158.4(4) . 33_545 ?
O75 Mo20 O5 87.6(4) . 33_545 ?
O46 Mo20 O21 96.4(4) . . ?
O76 Mo20 O21 87.4(4) . . ?
O75 Mo20 O21 158.2(4) . . ?
O5 Mo20 O21 84.2(4) 33_545 . ?
O46 Mo20 O83 170.7(4) . . ?
O76 Mo20 O83 82.1(4) . . ?
O75 Mo20 O83 81.0(4) . . ?
O5 Mo20 O83 76.7(4) 33_545 . ?
O21 Mo20 O83 77.5(4) . . ?
O46 Mo20 Mo18 99.4(3) . . ?
O76 Mo20 Mo18 47.8(3) . . ?
O75 Mo20 Mo18 47.6(3) . . ?
O5 Mo20 Mo18 135.0(2) 33_545 . ?
O21 Mo20 Mo18 135.0(3) . . ?
O83 Mo20 Mo18 89.8(3) . . ?
O79 Mo21 O72 104.7(4) . . ?
O79 Mo21 O26 104.8(4) . . ?
O72 Mo21 O26 93.3(4) . . ?
O79 Mo21 O78 97.0(4) . . ?
O72 Mo21 O78 86.8(4) . . ?
O26 Mo21 O78 157.3(3) . . ?
O79 Mo21 O16 96.2(4) . . ?
O72 Mo21 O16 158.1(4) . . ?
O26 Mo21 O16 87.6(3) . . ?
O78 Mo21 O16 84.1(3) . . ?
O79 Mo21 O81 170.8(4) . . ?
O72 Mo21 O81 81.5(4) . . ?
O26 Mo21 O81 81.4(4) . . ?
O78 Mo21 O81 76.2(3) . . ?
O16 Mo21 O81 77.1(4) . . ?
O79 Mo21 Mo19 99.7(3) . . ?
O72 Mo21 Mo19 47.8(3) . . ?
O26 Mo21 Mo19 47.9(3) . . ?
O78 Mo21 Mo19 134.2(3) . . ?
O16 Mo21 Mo19 135.3(2) . . ?
O81 Mo21 Mo19 89.6(2) . . ?
O55 Mo22 O36 103.7(5) . . ?
O55 Mo22 O71 104.8(5) . . ?
O36 Mo22 O71 92.7(4) . . ?
O55 Mo22 O20 97.6(5) . . ?
O36 Mo22 O20 157.9(4) . . ?
O71 Mo22 O20 87.6(4) . . ?
O55 Mo22 O33 96.2(5) . . ?
O36 Mo22 O33 88.2(4) . . ?
O71 Mo22 O33 158.1(4) . . ?
O20 Mo22 O33 83.6(4) . . ?
O55 Mo22 O57 170.5(4) . . ?
O36 Mo22 O57 82.5(4) . . ?
O71 Mo22 O57 81.8(4) . . ?
O20 Mo22 O57 75.7(4) . . ?
O33 Mo22 O57 76.6(4) . . ?
O55 Mo22 Mo3 99.1(4) . . ?
O36 Mo22 Mo3 47.2(3) . . ?
O71 Mo22 Mo3 47.8(3) . . ?
O20 Mo22 Mo3 135.0(3) . . ?
O33 Mo22 Mo3 135.0(3) . . ?
O57 Mo22 Mo3 90.3(3) . . ?
Mo11 Mo23 O18 170.2(12) . . ?
Mo11 Mo23 O21 79.9(9) . 33_545 ?
O18 Mo23 O21 106.4(7) . 33_545 ?
Mo11 Mo23 O34 78.9(9) . . ?
O18 Mo23 O34 106.0(7) . . ?
O21 Mo23 O34 105.9(7) 33_545 . ?
Mo11 Mo23 O1 77.1(8) . 2_655 ?
O18 Mo23 O1 94.4(6) . 2_655 ?
O21 Mo23 O1 150.1(8) 33_545 2_655 ?
O34 Mo23 O1 88.1(6) . 2_655 ?
Mo11 Mo23 O3 76.5(8) . 2_655 ?
O18 Mo23 O3 95.9(6) . 2_655 ?
O21 Mo23 O3 88.5(6) 33_545 2_655 ?
O34 Mo23 O3 148.6(8) . 2_655 ?
O1 Mo23 O3 67.8(4) 2_655 2_655 ?
Mo11 Mo23 O50 1.6(6) . . ?
O18 Mo23 O50 171.7(7) . . ?
O21 Mo23 O50 78.6(6) 33_545 . ?
O34 Mo23 O50 78.5(6) . . ?
O1 Mo23 O50 78.6(5) 2_655 . ?
O3 Mo23 O50 77.4(5) 2_655 . ?
Mo14 Mo24 O15 173.3(5) . . ?
Mo14 Mo24 O7 78.3(4) . . ?
O15 Mo24 O7 103.2(5) . . ?
Mo14 Mo24 O68 81.1(4) . . ?
O15 Mo24 O68 104.7(5) . . ?
O7 Mo24 O68 104.8(4) . . ?
Mo14 Mo24 O2 79.0(4) . . ?
O15 Mo24 O2 97.4(4) . . ?
O7 Mo24 O2 150.4(4) . . ?
O68 Mo24 O2 90.1(4) . . ?
Mo14 Mo24 O60 77.7(4) . . ?
O15 Mo24 O60 95.7(4) . . ?
O7 Mo24 O60 88.5(4) . . ?
O68 Mo24 O60 152.1(4) . . ?
O2 Mo24 O60 68.3(3) . . ?
Mo14 Mo24 O28 0.9(3) . . ?
O15 Mo24 O28 173.5(4) . . ?
O7 Mo24 O28 79.1(4) . . ?
O68 Mo24 O28 80.4(4) . . ?
O2 Mo24 O28 78.4(3) . . ?
O60 Mo24 O28 78.2(3) . . ?
Mo13 Mo25 O70 172.6(7) . . ?
Mo13 Mo25 O23 81.2(6) . . ?
O70 Mo25 O23 103.2(5) . . ?
Mo13 Mo25 O14 74.3(6) . . ?
O70 Mo25 O14 98.8(5) . . ?
O23 Mo25 O14 103.4(5) . . ?
Mo13 Mo25 O67 88.6(6) . . ?
O70 Mo25 O67 97.1(5) . . ?
O23 Mo25 O67 91.7(4) . . ?
O14 Mo25 O67 154.9(5) . . ?
Mo13 Mo25 O4 81.4(5) . . ?
O70 Mo25 O4 95.9(5) . . ?
O23 Mo25 O4 155.5(5) . . ?
O14 Mo25 O4 88.3(4) . . ?
O67 Mo25 O4 70.8(4) . . ?
Mo13 Mo25 O41 7.4(5) . . ?
O70 Mo25 O41 175.6(5) . . ?
O23 Mo25 O41 81.0(4) . . ?
O14 Mo25 O41 81.5(5) . . ?
O67 Mo25 O41 81.2(4) . . ?
O4 Mo25 O41 79.6(4) . . ?
Mo12 Mo26 O32 173.3(10) . . ?
Mo12 Mo26 O77 81.2(8) . . ?
O32 Mo26 O77 104.8(6) . . ?
Mo12 Mo26 O33 73.5(7) . . ?
O32 Mo26 O33 101.9(6) . . ?
O77 Mo26 O33 103.5(6) . . ?
Mo12 Mo26 O62 83.3(7) . . ?
O32 Mo26 O62 99.3(6) . . ?
O77 Mo26 O62 90.4(5) . . ?
O33 Mo26 O62 150.5(6) . . ?
Mo12 Mo26 O61 78.8(7) . . ?
O32 Mo26 O61 96.2(5) . . ?
O77 Mo26 O61 153.6(7) . . ?
O33 Mo26 O61 87.2(5) . . ?
O62 Mo26 O61 70.2(4) . . ?
Mo12 Mo26 O38 5.3(6) . . ?
O32 Mo26 O38 174.2(6) . . ?
O77 Mo26 O38 80.5(5) . . ?
O33 Mo26 O38 78.8(5) . . ?
O62 Mo26 O38 78.1(5) . . ?
O61 Mo26 O38 78.0(4) . . ?
Mo10 Mo27 O66 172.0(13) . . ?
Mo10 Mo27 O69 81.9(10) . . ?
O66 Mo27 O69 104.4(7) . . ?
Mo10 Mo27 O10 73.7(9) . . ?
O66 Mo27 O10 99.8(7) . . ?
O69 Mo27 O10 103.3(6) . . ?
Mo10 Mo27 O62 87.0(9) . . ?
O66 Mo27 O62 97.7(6) . . ?
O69 Mo27 O62 91.5(6) . . ?
O10 Mo27 O62 153.4(7) . . ?
Mo10 Mo27 O6 80.8(9) . . ?
O66 Mo27 O6 94.5(6) . . ?
O69 Mo27 O6 155.8(7) . . ?
O10 Mo27 O6 87.9(5) . . ?
O62 Mo27 O6 70.8(5) . . ?
Mo10 Mo27 O45 6.3(7) . . ?
O66 Mo27 O45 173.5(7) . . ?
O69 Mo27 O45 81.9(6) . . ?
O10 Mo27 O45 79.8(6) . . ?
O62 Mo27 O45 80.6(5) . . ?
O6 Mo27 O45 79.0(5) . . ?
O65 Mo28 O8 108.8(8) . . ?
O65 Mo28 O9 98.4(7) . . ?
O8 Mo28 O9 94.6(7) . . ?
O65 Mo28 O6 92.4(7) . . ?
O8 Mo28 O6 157.4(8) . . ?
O9 Mo28 O6 89.8(6) . . ?
O65 Mo28 O2 160.6(8) . . ?
O8 Mo28 O2 89.0(6) . . ?
O9 Mo28 O2 87.3(6) . . ?
O6 Mo28 O2 69.0(5) . . ?
O65 Mo28 O42 89.3(7) . . ?
O8 Mo28 O42 87.2(7) . . ?
O9 Mo28 O42 171.0(8) . . ?
O6 Mo28 O42 85.2(6) . . ?
O2 Mo28 O42 84.0(6) . . ?
Mo9 Mo29 O27 82.2(12) . . ?
Mo9 Mo29 O30 172.7(16) . . ?
O27 Mo29 O30 101.6(8) . . ?
Mo9 Mo29 O5 74.4(12) . . ?
O27 Mo29 O5 102.8(7) . . ?
O30 Mo29 O5 98.7(7) . . ?
Mo9 Mo29 O67 91.7(13) . . ?
O27 Mo29 O67 93.4(7) . . ?
O30 Mo29 O67 94.2(7) . . ?
O5 Mo29 O67 156.7(8) . . ?
Mo9 Mo29 O3 83.9(12) . . ?
O27 Mo29 O3 159.1(9) . . ?
O30 Mo29 O3 94.0(7) . . ?
O5 Mo29 O3 88.3(6) . . ?
O67 Mo29 O3 71.4(5) . . ?
Mo9 Mo29 O40 7.3(10) . . ?
O27 Mo29 O40 83.1(6) . . ?
O30 Mo29 O40 175.2(8) . . ?
O5 Mo29 O40 81.2(6) . . ?
O67 Mo29 O40 84.4(6) . . ?
O3 Mo29 O40 81.2(6) . . ?
C5 N14 H14A 120.0 . . ?
C5 N14 H14B 120.0 . . ?
H14A N14 H14B 120.0 . . ?
N11 C5 N13 121(4) . . ?
N11 C5 N14 122(5) . . ?
N13 C5 N14 115(4) . . ?
C5 N11 H11A 120.0 . . ?
C5 N11 H11B 120.0 . . ?
H11A N11 H11B 120.0 . . ?
C5 N13 H13A 120.0 . . ?
C5 N13 H13B 120.0 . . ?
H13A N13 H13B 120.0 . . ?

_refine_diff_density_max         1.805
_refine_diff_density_min         -4.054
_refine_diff_density_rms         0.303

_diffrn_radiation_source         synchrotron
_diffrn_radiation_monochromator  'Double Crystal Monochromator'
